1213ACI Structural Journal/September-October 2014
ACI STRUCTURAL JOURNAL TECHNICAL PAPER
Seven intermediate-scale slabs were constructed and tested to failure under sequential drop-weight impacts. The slabs contained longitudinal reinforcing bars and were constructed with steel fiber contents ranging from zero (that is, conventional rein-forced concrete) to 1.50% by volume. The data from the testing program were used to further assess the performance of steel fiber- reinforced concretes in impact-resistant applications and to provide a well-documented dataset pertaining to a research area which is currently limited within the literature. The test results showed that the addition of the steel fibers was effective in increasing slab capacity, reducing crack widths and spacings, and mitigating local damage under impact. Although the slabs in the program were designed to be flexure-critical under static loading conditions, the development of inertial forces under impact loading conditions led to observed responses and failure modes that were governed by shear.
Keywords: drop-weight impact; fiber-reinforced concrete; impact capacity; impact test; inertia; punching shear; steel fibers.
INTRODUCTIONThe behavior of reinforced concrete under impact is an
area of research that is still not well understood; however, work in this area continues to be motivated by a broad range of applications. Examples include reinforced concrete structures designed to resist accidental loading scenarios such as falling rock impact; vehicle or ship collisions with buildings, bridges, or offshore facilities; and structures that are used in high-threat or high-hazard applications, such as military fortification structures or nuclear facilities. As a result, considerable work has been undertaken in an effort to develop impact-resistant design procedures and to improve the performance of reinforced concrete structures subjected to impact loads.
To date, the majority of the impact-related research has been focused on developing empirical provisions to esti-mate member damage1,2 and capacity3 under specific types of impact-loading scenarios. When used to provide impact response estimates under conditions that differ from those considered in their development, the application of such formulae has been met with limited success.4 Moreover, with respect to wall and slab elements specifically, much of the work has been exclusively focused on localized damage mechanisms such as concrete scabbing, impactor (that is, missile) penetration, and impactor perforation.5-7 Although it is commonly accepted that reinforced concrete elements under impact generally respond in such a way that impact energy is dissipated through a combination of local damage development and global element deformations (bending, shear, and axial deformations),1 often little effort is focused
on studying the global response behaviors of reinforced concrete elements under impact.8
In recent decades, the use of fiber-reinforced concrete has emerged as a viable approach for improving the perfor-mance of concrete elements under impact. Several investi-gations have shown that compared with reinforced concrete, fiber-reinforced concrete elements containing traditional steel reinforcing bars (R/FRC elements) exhibit superior resistances to local damage development and, as a result, possess improved energy absorption capabilities under impact.9-11 As such, in the case of R/FRC elements, the global impact response can often be of greater significance than the formation of local damage mechanisms.
This paper presents the methodology and findings from an experimental program undertaken to investigate and document the impact behaviors of reinforced concrete (RC) and steel fiber-reinforced concrete slabs containing steel reinforcing bars (R/FRC slabs). Emphasis was placed on assessing the influence of end-hooked steel fibers on the measured slab behavior and, in contrast to much of the related experimental work available in the literature, on investigating the global dynamic impact responses of the slabs as well as local damage development. In an effort to fully capture the global impact behaviors, the slabs in this testing program were well-instrumented, and the test data collected were used to provide an openly accessible dataset that can be used by others to develop and assess related analytical procedures.
RESEARCH SIGNIFICANCEThere is growing realization of the need for resilient
structures and, as a result, a need for adequate, related assessment and design procedures. With respect to impact- resistant structures, the development of such procedures has been hindered by a lack of high-quality experimental data.4
This paper presents the performance and findings from an experimental program undertaken to investigate RC and R/FRC slabs under high-mass, low-velocity impact. Test data are used to assess the influence of steel fibers on impact response, to analyze global slab behavior, and to contribute to an area of research in which limited data are currently available.
Title No. 111-S103
Behavior of Steel Fiber-Reinforced Concrete Slabs under Impact Loadby Trevor D. Hrynyk and Frank J. Vecchio
ACI Structural Journal, V. 111, No. 5, September-October 2014.MS No. S-2013-161.R1, doi: 10.14359/51686923, was received September 12,
2013, and reviewed under Institute publication policies. Copyright 2014, American Concrete Institute. All rights reserved, including the making of copies unless permission is obtained from the copyright proprietors. Pertinent discussion including authors closure, if any, will be published ten months from this journals date if the discussion is received within four months of the papers print publication.
1214 ACI Structural Journal/September-October 2014
Specimen designSeven intermediate-scale slab specimens, identified as
Slabs TH2 through TH8, were constructed and tested under drop-weight impact (Fig. 1). Three slabs were constructed using plain concrete, and four slabs were constructed from a steel fiber-reinforced concrete (SFRC) mixture design with varied volumes of end-hooked steel fibers. Both concrete mixtures were adapted from 50 MPa (7.3 ksi) nominal cylinder-strength designs developed previously,12 and are reported in Table 1. Two parameters were varied amongst the slabs: the steel fiber volume fraction Vf, which ranged from zero to 1.5%, and the longitudinal reinforcement ratio rl, which was equal in the planar directions of the slabs and ranged from 0.273 to 0.592% per layer. The program test matrix is presented in Table 2.
The slabs were 1800 mm (71 in.) square, 130 mm (5.1 in.) thick, and were doubly reinforced with equal amounts of steel in the top and bottom mats of reinforcement, with each reinforcement mat being comprised of two orthogonal reinforcement layers. To accommodate different longitu-dinal reinforcement ratios, two types of reinforcing bars were used: No. 3 (U.S.) mild bars with cross-sectional areas of 71 mm2 (0.11 in.2) and nominal diameters of 9.5 mm (0.38 in.), and No.10M bars with cross-sectional areas of 100 mm2 (0.16 in.2) and nominal diameters of 11.3 mm (0.45 in.). Steel links constructed from bent No. 3 bars were used in the corner and center regions of the slabs to join the top and bottom reinforcement mats together. The typical longitudinal reinforcement layout is illustrated in Fig. 2.
The R/FRC slabs were constructed using end-hooked steel fibers with the following nominal properties: fiber length of 30 mm (1.18 in.), diameter of 0.37 mm (0.015 in.), aspect ratio of 80, and ultimate tensile strength of 2300 MPa
(330 ksi). The geometry of the end-hooked steel fiber used is illustrated in Fig. 3. Concrete material tests in the form of standard compression cylinders, bending prisms, and dog-bone shaped direct tension specimens were performed to characterize the mechanical properties of the concrete and to provide test data that are often required for the develop-ment of numerical models. Sample results illustrating the influence of the steel fibers on the compressive stress-strain responses of the concrete and the post-cracking tensile stress softening behaviors of the steel fiber-reinforced concrete are presented in Fig. 4. It should be noted that direct tension tests were not performed for the plain concrete; however, brittle responses characterized by rapid post-cracking strength loss were observed from the flexural testing of the plain concrete prisms. Mean mechanical properties developed from the concrete material tests and coupon tests of the steel rein-forcing bars are summarized in Table 3. Additional details regarding the material test specimens, the testing procedures used, and the response measurements obtained from each material test performed are available elsewhere.13
Fig. 1Drop-weight test frame.
Table 1Concrete dry mixture proportions
Water, kg/m3 (lb/yd3)
Cement, kg/m3 (lb/yd3)
(fl oz)SP*, mL(fl oz)
R*, mL(fl oz)
Plain 139 (234) 375 (632) 847 (1428) 1080 (1820) 1000 (33.8) 3500 (118) 488 (16.5)
SFRC 163 (275) 500 (843) 1114 (1878) 792 (1335) 2750 (93.0) 3500 (118) 650 (22.0)*CA = 13 mm (1/2 in.) crushed limestone coarse aggregate; WR is water reducer; SP is high-range water-reducing admixture; and R is retarder.79 kg/m3 (133 lb/yd3) steel fibers required per 1.0% fiber volume.
Table 2Test matrix
ment ratio rl*, %Reinforcing bar/spacing, mm (in.)
Fiber volume fraction Vf, %
TH2 0.420 No. 3/130 (5.1)
TH3 0.420 No. 3/130 (5.1) 0.50
TH4 0.420 No. 3/130 (5.1) 1.00
TH5 0.420 No. 3/130 (5.1) 1.50
TH6 0.273 No. 3/200 (7.9)
TH7 0.592 10M/13